and education use, including for instruction at the authors institution
and sharing with colleagues.
Other uses, including reproduction and distribution, or selling or
licensing copies, or posting to personal, institutional or third party
websites are prohibited.
In most cases authors are permitted to post their version of the
article (e.g. in Word or Tex form) to their personal website or
institutional repository. Authors requiring further information
regarding Elsevier’s archiving and manuscript policies are
encouraged to visit:
The role of notching damage on the fracture parameters of
ethylene-propylene block copolymers
, A. Segoviab
, A.B. Martínezb
, J. Rodrígueza
aDepartamento de Ciencia e Ingeniería de Materiales, Escuela Superior de Ciencias Experimentales y Tecnología, Universidad Rey Juan Carlos, C/Tulipán, s/n. 28933
Móstoles, Madrid, Spain
Centre Català del Plàstic-Universitat Politècnica de Catalunya, C/Colom, 144. 08222 Terrassa, Barcelona, Spain
a r t i c l e i n f o
Received 21 May 2010 Accepted 9 July 2010
Femtolaser and razor sharpening Damage
Ethylene-propylene block copolymer
a b s t r a c t
The inﬂuence of the notching procedure on the fracture toughness measured via Elastic-Plastic Fracture Mechanics has been analyzed on four different ethylene-propylene block copolymers with two distinct dimensions, paying special attention to the morphology of the area surrounding the crack tip front. Two sharpening techniques were evaluated: the traditional steel razor blade and the femtolaser ablation process. The fracture toughness of the razor blade sharpened samples was always higher than that of the femtolaser sharpened specimens. Also, the fracture toughness of the razor blade samples was dependent on the thickness of the samples, whereas the fracture toughness of the fem-tolaser sharpened specimens was not inﬂuenced by the dimensions of the test specimens. The microscopic analysis of non-tested samples showed that the crack tip radii were similar for both type of sharpened samples but the damage and its extension ahead of the crack tip was dependent on the notching technique, the copolymer type and the dimen-sions of the analyzed specimen. The femtolaser sharpened samples presented a very tiny heat affected zone ahead of the crack tip, the size of which was independent of the copolymer type and the dimensions of the test specimen. On the other hand, the steel razor blade sharpened samples showed an area surrounding the crack tip formed by plastic deformation, the length of which increased for the smaller size of sample and for higher ethylene content in the copolymer.
Ó2010 Elsevier Ltd. All rights reserved.
Recently, some works have appeared in the literature reporting the relevance of the notch sharpening technique when evaluating the fracture toughness of polymeric materials[1–4]. It is a well-known fact that the quality of the notch is of deciding importance to determine well established fracture toughness values using Linear Elastic Fracture Mechanics (LEFM), J–R resistance curves using Elastic-Plastic Fracture Mechanics (EPFM) or Essential Work of Fracture (EWF) parameters using Post Yielding
Fracture Mechanics (PYFM). Therefore, the notch sharp-ening procedure is crucial and tackled by both ESIS (Euro-pean Structural Integrity Society) [5–7] and ASTM International (Previously American Society for Testing and Materials)[8–10].
Martínez et al.[1,2]and Salazar et al.[3,4]have focused their research on the inﬂuence of the notch sharpening technique on the fracture parameters determined under LEFM[3,4], EPFM [3,4] and PYFM [1,2,4] conditions. The polymeric material utilized for their investigation was an ethylene-propylene block copolymer. The sharpening procedure was performed using steel razor blades and a femtosecond pulsed laser. The femtosecond pulsed laser ablation is characterized by very rapid creation of vapor *Corresponding author. Tel.:þ34 91 488 82 92; fax:þ34 91 488 81 50.
E-mail address:firstname.lastname@example.org(A. Salazar).
Contents lists available atScienceDirect
j o ur n a l ho m e p a g e : w w w . e l s e v i e r. c o m / l oc a t e / po l y t e s t
and plasma phases, negligible heat conduction and the absence of a liquid phase[11,12]. Hence, this technique can remove the material of the notch tip by ablating it with almost no heat dissipation, preventing melting and thermal deformation of the surrounding area. These works proved that, independently of the fracture mechanics conditions, the fracture toughness of the specimens sharpened through femtosecond laser ablation showed lower values compared to those obtained on the samples sharpened using a steel razor blade. These differences could range fromw10% up to 90% under LEFM and PYFM conditions, respectively. The damage produced ahead of the crack tip through plastic deformation in the steel razor blade sharpened samples seemed to be the reason of this increase in the fracture toughness.
To date, the reports found in the literature concerning the inﬂuence of the notch sharpening technique on the fracture parameters have been focused on the experi-mental notching procedure, regardless of the type of polymeric material. Also, they do not quantify the damage facing the crack front. For these reasons, the objective of the present work is to evaluate if the differences found in the fracture parameters between femtolaser and sharp razor blade notched specimens are held independently of the morphological and structural properties of the ethylene-propylene block copolymer. Hence, four ethylene-ethylene-propylene block copolymers with different structural properties have been chosen and the fracture parameters have been determined under EPFM conditions. Subsequently, the fracture toughness values are discussed in the light of the specimen thickness, the size and type of damage ahead of the crack tip and the structural parameters of the different copolymers.
2. Experimental procedure
The materials under study were four commercial grade ethylene-propylene block copolymers, EPBCs, supplied by Repsol in the form of pellets. The bulk specimens for frac-ture characterization were prepared by injection moulding. The basic characteristics such as the ethylene content and the isotactic index determined from Nuclear Magnetic Resonance (NMR), the glass transition temperatures cor-responding to the elastomeric particles,TgEPR, embedded in the propylene matrix, Tg PP, measured via Dynamic Mechanical Thermal Analysis (DMTA), and molecular weights obtained by Gel Permeation Chromatography (GPC) are collected inTable 1.
The mechanical properties such as the Young’s modulus, E, and the yield stress,
sY, were measured via tensile tests at a cross-head speed of 1 mm/min using ISO-527 bulk injected tensile samples (Table 2).
2.2. Sample preparation
Fracture toughness tests on bulk specimens were carried out on injected single edge notched bend specimens (SENB). For each copolymer, two specimen thicknesses, 6.35 mm and 9 mm, were analyzed, the overall dimensions being 6.3512.755 mm and 91880 mm, respectively. An initial straight-through slot with a depth to width ratio of 0.5 and terminating in aV-notch with 0.2 mm root radius was machined in all the specimens.
Two different procedures for the sharpening of the SENB specimens were carried out:
S-Type: The notch sharpening is performed with a fresh steel razor blade following the guidelines given by ESIS
F-Type: The sharpening of the notch is produced through femtosecond pulsed laser ablation (Femtolaser)[11,12], using a commercial Ti:sapphire oscillator (Tsunami, Spectra Physics) plus a regenerative ampliﬁer system (Spitﬁre, Spectra Physics) based on the chirped pulse ampliﬁcation (CPA) technique. 120-fs pulses at 795 nm with a repetition rate of 1 kHz were produced. The scanning speed was 130
mm/s and 8 passes were conducted with a pulse energy of 0.07 mJ. The sharp length inserted by the femtolaser was 500
The total initial crack depth, ao, to width ratio after sharpening was 0.55.
The morphology and dimensions of the crack tip after sharpening and the area beneath it of non-tested speci-mens were analyzed via light microscopy (Leica DMR) and scanning electron microscopy (Hitachi S-3400 N). Prepa-ration prior to examination consisted of sectioning the bulk copolymer intoﬁlms with thickness in the range between 6 and 10
mm with a microtome (Rotary Microtome Leica RM2265). The resulting sections were picked up and mounted on microscope slides to be analyzed via trans-mitted light microscopy or platinum sputter coated for scanning electron microscopy.
2.3. Fracture tests
The ESIS TC4 Protocol entitled “The determination of J-fracture toughness of polymers at slow speed”, was followed to achieve the J–R curves from multiple speci-mens. A minimum of seven samples was tested using an
Basic properties of the copolymers under study.
NMR DMTA GPC
Etylene content (%wt) Isotactic Index (%) TgPP (C) TgEPR (C) Mw(kg/mol) Mn(kg/mol) Mz(kg/mol) Polidispersity (Mw/Mn)
EPBC1 6.9 89.3 10.6 45.8 816 161 2245 5.09
EPBC5 8.5 85.4 10.4 49.3 353 66 1026 5.37
EPBC7 8.5 84.2 10.5 49.4 302 56 882 5.39
EPBC12 11.2 81.0 10.5 49.4 307 61 878 5.05
electromechanical testing machine (MTS Alliance RF/100) with a load cell of5 kN. The tests were performed at room temperature and under displacement control at a cross-head speed of 1 mm/min using a three-point bendﬁxture of 50.8 and 96 mm loading spans for the SENB specimens with 6.35 and 9 mm in thickness, respectively.
3. Results and discussion
The mechanical response of the four copolymers at 23C and at a cross-head speed of 1 mm/min was highly
non-linear and the multiple specimen method was applied to determine theJ-crack growth resistance curves.Figs. 1 and 2combine the R-curves of the S-Type and F-Type specimens with 6.35 and 9 mm in thickness, respectively. These plots also include the ﬁt of the J-crack growth resistance curve to the power lawJ¼C$
DaN, with N 1. Independently of the copolymer type and specimen dimensions, the resistance curves of F-Type are always below those of S-Type. Moreover, the rising part of the R-curves shows little differences between theS-Type and F-Type samples. On the other hand, according to theﬁtted curves, for the same notch sharpening procedure, there seems to be no great inﬂuence of the thickness on the resistance curves.
Fig. 3collects the fracture toughness,JIC, obtained from the resistance curves ofS-Type andF-Type specimens with 6.35 mm and 9 mm in thickness. For the computation of JIC values, the guidelines described by Hale et al.have been followed, where this critical value has been replaced by
Fig. 1. J–Rcurves forS-Type andF-Type specimens of (a) EPBC1, (b) EPBC5, (c) EPBC7 and (d) EPBC12 determined from 6.35 mm thick samples.
Mechanical properties of the ethylene-propylene block copolymers.
E (GPa) sY(MPa)
EPBC1 1.380.06 26.10.6
EPBC5 1.540.03 23.90.5
EPBC7 1.4110.008 23.030.04
a pseudo-initiation value J0.2, which deﬁnes crack resis-tance at 0.2 mm of the total crack growth. The size requirements for plane strain JICare given by:
B; a; Wa>25 J
where B is the thickness, W is the width and a is the initial crack length. The fracture toughness values are not in plane strain except for EPBC12S-Type 9 mm thick samples and EPBC5, EPBC7 and EPBC12F-Type 9 mm thick specimens. The fracture values of the specimens sharpened with a steel razor blade,S-Type, showed in all cases higher values of the energy for crack growth initiation than the samples sharpened with the femtosecond laser,F-Type. The differ-ences ranged from 13% for EPBC1 6.35 mm thick to 74% for EPBC5 6.35 mm thick.
Analysis ofFig. 3yields further information. As regards theF-Type samples, for almost all the copolymers (EPBC5,
EPBC7 and EPBC12), the fracture toughness of the speci-mens with 6.35 mm in thickness is the same as that of 9 mm thick samples. However, this tendency is not fol-lowed by EPBC1. In the case of the S-Type samples, the fracture toughness of the 6.35 mm thick specimens is higher than that of the 9 mm thick samples except for EPBC7.
With the aim of evaluating the differences between F-Type andS-Type sharpened specimens, between 5 and 10 ﬁlms withw8
mm in thickness were microtomed along the depth of theS-Type andF-Type sharpened samples for each copolymer before being tested. Figs. 4 and 5 show the micrographs obtained via transmitted light microscopy of the appearance of the crack tip and the area ahead of it for EPBC1S-Type andF-Type sharpened specimens 6.35 and 9 mm thick, respectively. The crack tip has been marked with an arrow, and the measurements carried out at high magniﬁcation indicated that, independently of the copolymer,
Fig. 2.J–Rcurves forS-Type andF-Type specimens of (a) EPBC1, (b) EPBC5, (c) EPBC7 and (d) EPBC12 determined from 9 mm thick samples.
sharpening procedure and dimensions, the values of the crack tip radius were similar and ranging between 1 and 2
mm. However, there is a dark area in the material facing the crack tip (outlined with dots) which extends deeper in theS -Type samples (Figs. 4a and 5a). This dark area is more difﬁcult to observe in theF-Type specimens and, if it exists, it is conﬁned to a very tiny region ahead of the crack tip (Figs.
4b and 5b). Moreover, the dotted zone of the S-Type 6.35 mm thick specimens (Fig. 4a) seems to be bigger than that of theS-Type 9 mm thick specimens (Fig. 5a). This contrasts with the analysis of theF-Type samples as a func-tion of the thickness (Figs.4b and5b), because this tendency with the thickness could not be detected. To assess these trends, the damage length, measured as the length of a straight line going from the crack tip to the end of the dark area, was determined along the depth of the EPBC1S-Type andF-Type specimens with 6.35 and 9 mm in thickness. The resulting proﬁles were plotted inFig. 6a and b, respectively. As can be observed, the light microscopic inspection agrees with the measurements of the damage length. Indepen-dently of the specimen thickness and the analyzed depth, the damage length of theS-Type samples is always higher than that of theF-Type. Furthermore, the damage length of theS-Type 6.35 mm thick samples is greater than that of the S-Type 9 mm thick specimens, whereas for the F-Type
Fig. 3. Fracture toughness values, JIC, of EPBC1, EPBC5, EPBC7 and EPBC12 as
a function of the specimen’s thickness and the notching procedure.
Fig. 4. Micrographs of EPBC1 showing the crack tip of non-tested (a)S-Type
and (b)F-Type sharpened specimens with 6.35 mm in thickness. The arrow points out the end of the crack tip and the damage produced by plastic deformation is outlined by a dotted line.
Fig. 5.Micrographs of EPBC1 showing the crack tip of non-tested (a)S-Type
samples the damage length is not inﬂuenced by the spec-imen dspec-imensions.
The evolution of the damage ahead of the crack tip for non-tested EPBC1, EPBC5, EPBC7 and EPBC12 as a function of the notching procedure is collected inFigs. 7a and b for the specimens with 6.35 and 9 mm in thickness, respec-tively. The plots represent the average damage length, obtained from the analysis of the ﬁlms microtomed through the depth of the samples, together with their corresponding standard deviation. In the case of EPBC5, EPBC7 and EPBC12 copolymers, the damage ahead of the crack tip evolved similarly with the notching procedure and specimen thickness to that described for EPBC1. Several conclusions can be drawn from the analysis of theseﬁgures. Firstly, the length of the damage ofS-Type is always higher than that ofF-Type independently of the copolymer and specimen thickness. Furthermore, the damage length for
theF-Type specimens is inﬂuenced neither by the copol-ymer type nor the specimen dimensions. These quantita-tive results are in agreement with previous works[9,10]. It has been demonstrated that the region ahead of the crack tip with different texture to the rest of the virgin surface is caused during the notch sharpening.
To reach a better understanding of the nature of the damage ahead of the crack tip,S-Type andF-Type micro-tomedﬁlms were analyzed via scanning electron micros-copy.Figs. 8 and 9show the area surrounding the crack tip for EPBC5S-Type and F-Type sharpened samples, respec-tively. The main difference in the zone beneath the crack is the morphology of the damage. In theS-typeﬁlms, the area surrounding the crack tip is extremely deformed (Fig. 8a), with highly distorted holes left by the strained ethylene particles (Fig. 8b). These deformed particles can leave holes with up to 5
mm in length, which is a huge increase in size
Fig. 7.Damage length as a function of the notching technique for non-tested
EPBC1, EPBC5, EPBC7 and EPBC12 copolymers with (a) 6.35 and (b) 9 mm in thickness. 0 50 100 150 200
3 3,5 4 4,5 5 5,5 EPBC1 6.35 mm thick
S-Type F-Type ( ht g n el e g a m a d µ ) m depth (mm)
a0 50 100 150 200
4 4,5 5 5,5 6 6,5 7 7,5 EPBC1 9 mm thick
S-Type F-Type ( ht g n el e g a m a d µ ) m depth (mm)
Fig. 6. Evolution of the damage length ahead of the crack tip through the
specimen’s depth with the notching procedure for non-tested EPBC1 copolymers with (a) 6.35 mm and (b) 9 mm in thickness.
taking into account that the non stressed elastomeric particle dimension isw0.4
mm. On the other hand, the F-Typeﬁlms present a very small area affected by the heat dissipation (Fig. 9a) where partially melted zones produced by the pulses of the laser ablation process can be discerned (Fig. 9b). It is worth mentioning that some of theF-Type analyzedﬁlms were characterized by complete absence of damage ahead of the crack tip (Figs.4b and5b).
During the sharpening procedure with the fresh steel razor blade, the force of tapping acts along the depth which leads to stresses which exceed the yield stress locally and generate wide plastic deformation areas. The extension of these areas is higher as the depth of the specimen decreases, assuming that roughly the same force is applied independently of the thickness of the sample.
Apart from that, the damage length seems to be related to the structural parameters of the copolymer, especially with the ethylene content. Interestingly, the damage ahead of the crack tip of theS-Type samples increased as the amount of ethylene content in the copolymer was raised (Table 1). As the ethylene content is increased, the stiffness and yield stress are reduced (Table 2). This implies a softening of the copolymer with the addition of ethylene. Hence, if the same force is applied for all the samples, independently of the thickness and the type of copolymer, the resulting damage will be larger for higher ethylene content. On the other hand, in the F-Type
specimens, there is no physical contact with the specimen during the notching procedure, which is the reason why the damage dimensions are held constant independently of the copolymer and thickness of the specimen. The nature of the damage is conﬁned to a tiny heat affected zone.
Consequently, the presence of plastic deformation, either large (6.35 mm thick specimens) or small (9 mm thick specimens), accounts for the differences in the JIC values of the distinct sharpened specimens when measured within the EPFM regime. The energy necessary to start crack growth is higher when the crack tip encounters a deformed area (S-Type) than when encoun-tering almost virgin material (F-Type) because of the different mechanical properties of the crack front matter
[9,10]. However, for theS-type samples, the extension of the plastic deformation damage ahead of the crack tip clearly plays an important role in the fracture toughness values. It seems that the higher the damage length beneath the crack tip, the more energy is needed for the crack to start growing because the area affected by strain hardened material with different properties to the virgin material is larger. This can partly explain the differences in the fracture toughness values between the S-Type samples with 6.35 mm and 9 mm in thickness (Fig. 3).
Finally, concerning the stable crack growth resistance, the similarity in the rising part of the resistance curves
Fig. 9.Micrographs obtained via scanning electron microscopy showing the
morphology of the damage beneath the crack tip in EPBC5F-Type samples: (a) detail of the crack tip front and (b) damage ahead of the crack tip. The arrow points out the end of the crack tip.
Fig. 8. Micrographs obtained via scanning electron microscopy showing the
between theS-Type andF-Type samples independently of the copolymer type and dimensions (Figs. 1 and 2) is indication that the notching procedure only inﬂuences the crack growth initiation and not its consequent propagation.
The inﬂuence of the notching procedure on the fracture parameters obtained via EPFM has been analyzed in four different ethylene-propylene block copolymers with two distinct dimensions. The crack growth initiation energy of the specimens sharpened via traditional steel razor blade was always higher than that of the samples sharpened via the femtolaser ablation technique. Furthermore, for the razor blade samples, the fracture toughness was dependent on the thickness of the samples, being lower in the thicker specimens; whereas for the femtolaser sharpened speci-mens the fracture toughness was not inﬂuenced by the dimensions of the test specimens. The damage in the crack front accounts for the fracture toughness values as all the test samples presented similar crack tip radii. The damage produced during the sharpening with steel razor blade consisted of a highly plastically deformed area surrounding the crack tip, the extent of which was larger as the thick-ness of the samples was reduced and the ethylene content in the copolymer was increased. On the contrary, the damage of the femtolaser sharpened samples was conﬁned to a very tiny heat affected zone independently of the copolymer type and dimensions. Finally, the crack growth resistance was not affected by the notching procedure as the rising part of theJ–Rcurves was similar independently of the notching technique and the thickness of the samples.
Authors are indebted toMinisterio de Educaciónof Spain for their ﬁnancial support through the project MAT2009-14294, to REPSOL YPF for the materials supply and to PhD Pablo Moreno from theUniversidad de Salamanca for the femtolaser notching of the specimens.
A. Segovia thanks the National Council of Science and Technology (CONACYT) of Mexico, for the support of a doctoral research scholarship.
 A.B. Martínez, A. Segovia, J. Gámez-Pérez, M. Ll. Maspoch, Inﬂuence of femtolaser notch sharpening technique in the determination of essential work of fracture (EWF) parameters, Eng. Fract Mech. 16 (2009) 2604.
 A.B. Martínez, A. Segovia, J. Gámez-Pérez, M. Ll. Maspoch. Essential work of fracture analysis of the tearing of a ductile polymerﬁlm. Eng Fract Mech, Submitted for publication.
 A. Salazar, J. Rodríguez, A. Segovia, A.B. Martínez, Inﬂuence of the notch sharpening technique on the fracture toughness of bulk ethylene-propylene block copolymers, Polym. Test. 29 (2010) 49.  A. Salazar, J. Rodríguez, A. Segovia, A.B. Martínez, Relevance of the
femtolaser notch sharpening to the fracture of ethylene-propylene block copolymers, Eur. Polym. J. (2010). doi:10.1016/j.eurpolymj. 2010.06.012.
 J.G. Williams, KCand GCat slow speeds for polymes. in: D.R. Moore,
A. Pavan, J.G. Williams (Eds.), Fracture Mechanics Testing Methods for Polymers, Adhesives and Composites. Elsevier Science Ltd. and ESIS, The Netherlands, 2001, pp. 11–24.
 G.E. Hale, F. Ramsteiner, J-fracture toughness of polymers at slow speed. in: D.R. Moore, A. Pavan, J.G. Williams (Eds.), Fracture Mechanics Testing Methods for Polymers, Adhesives and Composites. Elsevier Science Ltd. and ESIS, , The Netherlands, 2001, pp. 123–157.  E. Clutton, Essential work of fracture. in: D.R. Moore, A. Pavan, J.G. Williams (Eds.), Fracture Mechanics Testing Methods for Polymers, Adhesives and Composites. Elsevier Science Ltd. and ESIS, , The Netherlands, 2001, pp. 177–195.
 ASTM E1820–06: Standard Test Method for Measurement of Frac-ture Toughness (2007).
 ASTM D5045–99: Standard Test Methods for Plane-Strain Fracture Toughness and Strain Energy Release Rate of Plastic Materials (1999).
 ASTM D6068–96: Standard Test Method for Determining J-R Curves of Plastic Materials (2002).
 B.N. Chichkov, C. Momma, S. Nolte, F. von Alvensleben, A. Tünner-mann, Femtosecond, picoseconds and nanosecond laser ablation of solids, Appl. Phys. A . Mater. 63 (1996) 109.
 P. Moreno, C. Méndez, A. García, I. Arias, L. Roso, Femtosecond laser ablation of carbon reinforced polymers, Appl. Surf. Sci. 252 (2006) 4110.
 J.G. Williams, Introduction to elastic-plastic fracture mechanics. in: D.R. Moore, A. Pavan, J.G. Williams (Eds.), Fracture Mechanics Testing Methods for Polymers, Adhesives and Composites. Elsevier Science Ltd. and ESIS, The Netherlands, 2001, pp. 119–122.  E.P. Moore, Polypropylene Handbook. Carl Hanser Verlag, Germany,